General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.56 - 7.7 g/cm³ Show Material materials with Density of 7.56 - 7.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | 20.0 °C | 215 - 218 GPa Show Material materials with Elastic modulus of 215 - 218 GPa | |

100.0 °C | 212 - 213 GPa Show Material materials with Elastic modulus of 212 - 213 GPa | ||

200.0 °C | 205 - 206 GPa Show Material materials with Elastic modulus of 205 - 206 GPa | ||

300.0 °C | 198 - 200 GPa Show Material materials with Elastic modulus of 198 - 200 GPa | ||

400.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | ||

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | ||

600.0 °C | 167 GPa Show Material materials with Elastic modulus of 167 GPa | ||

700.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | ||

Elongation | 20.0 °C | 12 % Show Material materials with Elongation of 12 % | |

Elongation A80 | 20.0 °C | 12 % Show Material materials with Elongation A80 of 12 % | |

Hardness, Brinell | 20.0 °C | 280 [-] Show Material materials with Hardness, Brinell of 280 [-] | |

Hardness, Rockwell B | 20.0 °C | 100 [-] Show Material materials with Hardness, Rockwell B of 100 [-] | |

Hardness, Vickers | 20.0 °C | 280 [-] Show Material materials with Hardness, Vickers of 280 [-] | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Martensitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Martensitic Stainless Steel |

Tensile strength | 20.0 °C | 850 - 900 MPa Show Material materials with Tensile strength of 850 - 900 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 20.0 °C | 9.9E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.9E-6 1/K | |

100.0 °C | 1.03E-5 - 1.05E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.03E-5 - 1.05E-5 1/K | ||

200.0 °C | 1.08E-5 - 1.1E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 - 1.1E-5 1/K | ||

300.0 °C | 1.1E-5 - 1.12E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.1E-5 - 1.12E-5 1/K | ||

400.0 °C | 1.15E-5 - 1.16E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 - 1.16E-5 1/K | ||

500.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

600.0 °C | 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.21E-5 1/K | ||

700.0 °C | 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 1/K | ||

800.0 °C | 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1370 - 1530 °C Show Material materials with Melting point of 1370 - 1530 °C | Typical for Martensitic Stainless Steel | |

Specific heat capacity | 20.0 °C | 450 - 460 J/(kg·K) Show Material materials with Specific heat capacity of 450 - 460 J/(kg·K) | |

100.0 °C | 482 J/(kg·K) Show Material materials with Specific heat capacity of 482 J/(kg·K) | ||

200.0 °C | 506 J/(kg·K) Show Material materials with Specific heat capacity of 506 J/(kg·K) | ||

300.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

400.0 °C | 547 J/(kg·K) Show Material materials with Specific heat capacity of 547 J/(kg·K) | ||

500.0 °C | 576 J/(kg·K) Show Material materials with Specific heat capacity of 576 J/(kg·K) | ||

600.0 °C | 616 J/(kg·K) Show Material materials with Specific heat capacity of 616 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 16 - 30 W/(m·K) Show Material materials with Thermal conductivity of 16 - 30 W/(m·K) | |

100.0 °C | 17.2 W/(m·K) Show Material materials with Thermal conductivity of 17.2 W/(m·K) | ||

200.0 °C | 18.6 W/(m·K) Show Material materials with Thermal conductivity of 18.6 W/(m·K) | ||

300.0 °C | 20 W/(m·K) Show Material materials with Thermal conductivity of 20 W/(m·K) | ||

400.0 °C | 21.2 W/(m·K) Show Material materials with Thermal conductivity of 21.2 W/(m·K) | ||

500.0 °C | 22.3 W/(m·K) Show Material materials with Thermal conductivity of 22.3 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.1 W/(m·K) Show Material materials with Thermal conductivity of 24.1 W/(m·K) | ||

800.0 °C | 25.5 W/(m·K) Show Material materials with Thermal conductivity of 25.5 W/(m·K) | ||

900.0 °C | 26.9 W/(m·K) Show Material materials with Thermal conductivity of 26.9 W/(m·K) | ||

1000.0 °C | 28.3 W/(m·K) Show Material materials with Thermal conductivity of 28.3 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | |

100.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

200.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.4 mm²/s Show Material materials with Thermal diffusivity of 4.4 mm²/s | ||

500.0 °C | 4.1 mm²/s Show Material materials with Thermal diffusivity of 4.1 mm²/s | ||

600.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 6.5E-7 - 9.06E-7 Ω·m Show Material materials with Electrical resistivity of 6.5E-7 - 9.06E-7 Ω·m |

100.0 °C | 9.42E-7 Ω·m Show Material materials with Electrical resistivity of 9.42E-7 Ω·m | |

200.0 °C | 9.87E-7 Ω·m Show Material materials with Electrical resistivity of 9.87E-7 Ω·m | |

300.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

400.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

500.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

600.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

700.0 °C | 1.22E-6 Ω·m Show Material materials with Electrical resistivity of 1.22E-6 Ω·m | |

800.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

900.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

1000.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.45 - 0.55 % Show Material materials with Carbon of 0.45 - 0.55 % |

Chromium | 14 - 15 % Show Material materials with Chromium of 14 - 15 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Molybdenum | 0.5 - 0.8 % Show Material materials with Molybdenum of 0.5 - 0.8 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |

Vanadium | 0.1 - 0.2 % Show Material materials with Vanadium of 0.1 - 0.2 % |